The INRAR Working Paper Series
The International Network for Bamboo and Rattan (INBAR) is a network of scientists anddevelopment workers from universities, governments and, increasingly, NGOs, who areworking on various aspects of bamboo and rattan. The principal objectives of the network are :to improve the well-being of small-scale producers and users of bamboo and rattan within thecontext of a sustainable bamboo/rattan resource base; to build skills and enhance capacityof national programmes to expand/orient bamboo and rattan research consistent with thepriorities identified; and, to strengthen national, regional and international coordination,cooperation, and collaboration.
INBAR seeks to accomplish its goals by identifying and supporting research consonant withthe priorities identified by national programmes. There is a strong emphasis on collaborativeapproaches to address problems which have regional and international relevance. Thenetworks research and development activities are organised according to five themes : Socio-economics Research; Production Research; Post-Harvest Technology Research; Biodiversityand Genetic Conservation (jointly with the International Plant Genetic Resources Institute(IPGRI) and Information, Training, and Technology Transfer.
Communication is vital to any network. INBAR uses a variety of fora, including a quarterlynewsletter, the INBAR Technical Reports Series, and this, the Working Paper Series.
The INBAR Working Paper Series is designed to promote the rapid exchange of informationon various aspects of bamboo and rattan science, and on the applications of research forsustainable development. The papers may be generated within INBAR research projects.However, other papers relevant to INBARs mandate and objectives are welcomed, and will begiven due consideration for publication.
INBAR was established with financial support from the International Development ResearchCentre (IDRC) of Canada and the International Fund for Agricultural Development (IFAD),based in Rome. The network is managed by IDRC and based at IDRCs South Asia RegionalOffice in New Delhi, India.
For further information on INBAR please contact :
The INBAR SecretariatC/o IDRC (SARO)17 Jor Bagh,New Delhi-l 10 003,INDIA.Tel. : (91-11) 461-941 l/464-4493Fax : (91- 11) 462-2707e-mail : Cherla@IDRC.ernet.in/SCherla@idrc.ca
BENDING STRENGTH OF GUADUA BAMBOOCOMPARISON OF DIFFERENT TESTING PROCEDURES
R. GNANAHARANKerala Forest Research Institute, India
JULES J. A. JANSSENOSCAR ARCE*
Technical University of Eindhoven, Netherlands(*Presently at Costa Rica Institute of Technology, Costa Rica)
Kerala Forest Research Institute, IndiaInternational Network for Bamboo and Rattan
a n dInternational Development Research Centre, Canada
INBAR Working Paper No. 3
KERALA FOREST RESEARCH INSTITUTE Peechi 680 653, India
INTERNATIONAL DEVELOPMENT RESEARCH CENTRE, CANADA17, Jor Bagh, New Delhi 110 003, India
All rights reserved. No part of this publication may be reproduced or transmit-ted in any form or by any means, electronical or mechanical, includingphotocopy, recording or any information storage and retrieval system, withoutpermission in writing from the publisher.
KFRI Library Cataloguing in Publication Data
GNANAHARAN, R. et al.Bending strength of bamboo: Comparison ofdifferent testing procedures with a view tostandardization. Peechi: KFRI and IDRC;New Delhi, 1994.
1. Bamboo - bending strength. 2. Bendingtesting procedure - bamboo.
In the context of diminishing natural resources, bamboo has emergaed as a viablealternative to wood, not only on account of its quick renewability, but its unique propertiesalso - both physical and mechanical. Its potential as an engineering material is thereforereceiving increasing attention.
To exploit its potential as an engineering material on an enduring basis, architects,engineers and users will need to be convinced of its suitability via Standards - national andinternational, building codes, etc. Although the structure and properties of a large numberof bamboo species have been investigated, the information has largely remained restrictedin its importance to biologists only. As methods of testing bamboo for its strength propertieshave not been standardized, the wealth of information on properties already available cannotbe utilized to promote engineering applications. This was forcefully articulated in the CochinInternational Bamboo Workshop (1988) and as a follow up, the International DevelopmentReseach Centre (IDRC) coordinated with the Technical University of Eindhoven (TUE),Netherlands and brought out the annotated bibliography on bamboo as an engineeringmaterial (199 1). In the Chiangmai Workshop (199 l), the immediate need to develop Standardsand Building Codes was stressed. This study is a beginning in that direction.
This intensive investigation, although confined to a new world bamboo species viz :Guadua angustifolia from Costa Rica in respect to just one important property, i.e., bendingstrength, has helped in confirming that strength values vary significantly depending on theform (round or split), span and position of skin surface of test specimens. Hence, it is clearthat apart from parameters like age, moisture content, position in culm, distribution of node,etc., standardization of form, span and position of skin surface of the test procedures whichwill ensure replication of results, comparison of values and reliability in engineering applica-tions.
This study is the result of collaborative effort between the Technical University ofEindhoven, Netherlands and Kerala Forest Research Institute, India. My sincere thanks toProf. Jules J.A. Janssen, a long time adviser to IDRC in bamboo research, for making thiscollaborative study possible and to Dr. R. Gnanaharan for undertaking the research.
New Delhi Cherla B. SastryMarch, 1995 Program Director; INBAR
Sincere thanks are due to the International Development Research Centre, Canada(IDRC) for sponsoring the first author to study at the Technical University of Eindhoven, theNetherlands (TUE), 12 April- 14 May 1993. Our sincere appreciation is due to Dr. Cherla B.Sastry. Principal Programme Officer, IDRC, for his keen interest in the collaborative studyand his active support.
The Board of the TUE willingly provided free office space and laboratory and technicalassistance to the first author.
Sincere appreciation is due to Dr. S. Chand Basha, Former Director, Kerala ForestResearch Institute (KFRI) and the Executive Committee of KFRI for allowing the first authorto u.ndertake the study.
The bending tests could not have been carried out without the able assistance of Mr. EricWyen, Research Assistant. Mr. Huub Donders, Carpenter, helped in the preparation of testspecimens of split bamboo. Mr. Ben Elfrink, Photographer, processed all the photographswithin a tight deadline. Mr. Sip Overdyk, Head of the Laboratory, provided all the neededassistance. Our sincere appreciation goes to all of them.
Valuable statistical advice was given by Dr. K. Jayaraman of KFRI. Mrs. C. Sunanda andMr. V. Sreekumar helped in carrying out the analysis and the latter also helped in arrivingat the prediction models.
Ms. P.K. Sugatha Devi diligently did the word-processing. Mr. K.K. Ramakrishnan andMr. V. Asokan ably handled the DTP work.
*INBAR would like to thank Drs. Trevor Williams and Canapathy for their editorial inputs.
( iii )
Bamboo, the fastest growing woody plant, has attracted the attention of not onlybiologists but also engineers and architects. Strength data are lacking for most species. Evenavailable data are difficult to compare because different testing procedures have been usedby different authors. Standardizing the testing procedures is essential to eventually arrive ata Bamboo Building Code. Towards this objective, a collaborative study between the KeralaForest Research Institute, India (KFRI) and the Technical University of Eindhoven, theNetherlands (TUE) was undertaken.
Straight, large diameter culms of Guadua angustifolia were used in the study. Different
types of test specimens were evaluated. Round, long specimens were subjected to 4-pointbending tests with a span of 3000 mm while round, short specimens to 3-point bending testswith a span of 700 mm. Split specimens were subjected to 3-point bending, and half thenumber of specimens was tested with skin surface in tension and the other half with skinsurface in compression. Strength properties like modulus of rupture (MOR) and modulus ofelasticity (MOE) were determined and the data were analyzed statistically. Salient findings ofthe study are given below:
MOR and MOE values obtained from the tests using three different types of specimens(round, long; round, short; split) are significantly different from each other.
Bending tests of round, short specimens with span length in the order of 700 mm do notreflect the actual potential of bamboo. In short-span testing, the specimens are not subjectedto true bending.
Density and outer diameter, in combination, can be successfully used in predicting theMOR and MOE of long specimens (R2 values of 0.994 and 0.989 respectively). This needs tobe confirmed by carrying out tests on long specimens of different bamboo species of large,medium, and small diameter.
The strength values of long members are evaluated by the 4-point test but this iscumbersome. This report shows that using some physical properties, strength can bepredicted. This needs to be tested in other species.
C O N T E N T S